Esthetic and functional consideration in restoring endodontically treated teeth
Esthetic andFunctionalConsiderationin RestoringEndodonticallyTre a t e d Te e t hRichard D. Trushkowsky, DDS* KEYWORDS Endodontics Ceramic Post RestorationThe selection of the best restoration for an endodontically treated tooth in theaesthetic zone1 depends on strength and the ability to recreate the form, function,and aesthetics of the natural tooth.2 The increased use of all-ceramic materials isa result of improved ceramic materials and adhesive systems.3 However, the adventof the current variety of translucent ceramic systems makes the shade of the abutmentimportant in achieving the desired aesthetic outcome. Carossa and colleagues4studied different posts and cores and thought that, although there were significantdifferences spectrophotometrically, clinically these differences were not noticeable.Deger and colleagues,5 Vichi and colleagues,6 and Nakamura and colleagues7 arrivedat different conclusions. They found that translucent ceramic crowns thinner than1.6 mm are affected by the color of the core. Vichi and colleagues6 found that whenthe thickness of the ceramic crown was 1 mm, color differences with the adjacentteeth are visually noticeable. Color differences decreased when the thickness wasincreased to 1.5 mm, and at 2.0 mm, no differences were noticeable. Michalakisand colleagues8 found that cast posts can result in root discoloration and havea blue-gray effect if the overlying bone and soft tissue are thin, which would be espe-cially important if a high lip line or broad smile exposes the restoration. De Rouffignacand de Cooman9 suggested using cast metal posts and cores with 2 thin metal tags toretain a ceramic for the core. However, this only addressed the optical effects in the The author has nothing to disclose. Department of Cariology and Comprehensive Care, New York University College of Dentistry, 345 East 24th Street, New York, NY 10010, USA * 483 Jefferson Boulevard Staten Island, NY 10312-2332. E-mail address: ComposiDoc@aol.com Dent Clin N Am 55 (2011) 403–410 doi:10.1016/j.cden.2011.01.009 dental.theclinics.com 0011-8532/11/$ – see front matter Ó 2011 Elsevier Inc. All rights reserved.
404 Trushkowsky coronal aspect, not in the root. If cast gold is used for the post and core, Carossa and colleagues4 found greater luminance with a polished core compared with a matte- finished one. Because the shade of the final restoration is affected by the color of the abutment, the need for a post and the nature of the post must be considered. Previously, a post was considered necessary for reinforcing an endodontically treated tooth, but most recent studies demonstrate a weakening effect rather than reinforcement.10 Some clinicians feel that the use of adhesive materials allow the clinician to bond the post to the dentin, the core to the post, and the ultimate restoration to the post-core and remaining tooth structure. Theoretically, when the various components with analo- gous properties are bonded together, the root can be strengthened, but this theory has not been proved.11 However, when there is insufficient tooth structure present, full coverage restorations may need a post to provide adequate retention.12 NEED FOR A POST Post preparation may increase the risk of root fracture.13 Teeth that have been debil- itated by trauma, caries, or previous restoration are often those that require endodontic treatment. Endodontic access forms require straight-line entrance and the “crown down” technique requires adequate removal of both coronal and radic- ular dentin to provide a continuously tapered preparation to the apex. The remaining tooth structure needs to be evaluated on its ability to retain and support the final restoration. The type of post and adhesive system that provides the best strength, reliability, aesthetics, and ease of handling should be selected.14 Peroz and colleagues15 formulated a classification of the amount of remaining tooth structure that is related to the remaining walls. Class I has all 4 axial walls remaining and only the access preparation, class II has 1 cavity wall removed and could be either an mesial-occlusal or distal-occlusal. Class III is an mesial-occlusal-distal cavity with 2 remaining walls, and class IV has only 1 remaining wall (either a buccal or lingual). Class V has no remaining walls. Dietschi and colleagues16 delineated the modifica- tions that occur in dentin composition, physical characteristics, fracture resistance, tooth stiffness, and restorative materials and techniques that would be required to effectively restore an endodontically treated tooth. He also determined that there is a change in not only the water content but also the Young modulus, and propor- tional limit are modified slightly. There is no resulting decrease in compressive strength and tensile strength. TYPES OF POSTS Zirconia posts were introduced by Meyenberg and colleagues17 in 1993. Prefabri- cated zirconia posts possess some positive attributes such as high strength to bending forces and good optical properties. However, their use with pressed ceramic or composite resin cores has been problematic because of delamination. One-piece milled zirconia post and core eliminates this dilemma, as there is no interface between the post and core. In addition, the diameters of the posts available limit their use in smaller-diameter teeth such as mandibular incisors, lateral incisors, and maxillary first premolars. Zirconia posts also possess a high modulus of elasticity (200 GPa). Some clinicians think that stiffer posts and cores allow increased support for the final resto- ration and create a more uniform distribution of stress. Others think that a more flexible post would be more beneficial, as bending under load causes loss of the restoration but allows the root system to be accessible for a new restoration. Micromotion of the post and core may result in failure of the luting cement, coronal leakage, and
Restoring Endodontically Treated Teeth 405recurrent decay.18 Zirconium posts are not recommended for posterior teeth becauseof the higher occlusal forces. In the anterior region, average forces are 222 N, andposts and cores have to be able to withstand these forces.19 Zirconia posts are rigid and hard and may cause disastrous fractures of the root; ifthe post fractures, it would be extremely difficult to remove. Zirconium oxide ceramicsalso undergo phase transformation at different temperatures. The addition of yttriumoxide to zirconium oxide creates a partially stabilized ceramic (yttria partially stabilizedzirconia [YPSZ]). When a crack is initiated in YPSZ with metastable tetragonal grains,the materials high fracture resistance reduces the chance of the crack propagating.Another potential problem is related to fit. The one-piece zirconium posts may havea passive fit relative to the acrylic resin patterns and after adjusting the posts, althoughnot binding did not fit accurately.Nonrigid Post Systems Carbon fiber Glass fiber Quartz fiber Silicon fiber. Fiber posts were introduced in 1990 and were made of carbon fiber. The carbonfibers were arranged longitudinally and surrounded by an epoxy matrix. These postshad a modulus of elasticity that was supposed to be close to that of dentin and mayprovide a more uniform distribution of stress on the remaining root structure. Unfortu-nately, these posts were radiolucent, and the dark color was detrimental to the shadeof ceramic crowns.6 Although fiber posts possess several advantages, there are alsodisadvantages. Because the modulus of elasticity and flexural strength are similar tothat of dentin, occlusal load may result in flexure, possibly resulting in micromovementand subsequently coronal leakage, caries, and loss of the restoration. The presence ofa sufficient ferrule reduces the chance of this occurring.20 However, debonding of thepost has been the main cause of failure of restorations in which the post was utilized.Some studies have indicated that an increased volume of cement around the post,especially at the coronal level, may result in loss of retention. Ideally, a thin, uniformcement layer would be beneficial for retention, which can be achieved only witha well-fitting post. A passive post should not transmit stress to the root. Therefore,the fit of the post and the thickness of the cement layer have to be considered to avoidstress transmission to the root.21 Because most canals are not circular, the use ofa preformed post requires modification of canal anatomy, and often the removal ofsound dentin, to accommodate the post. The use of an undersized post increasesthe cement volume and possibly increases the rate of debonding. The clinician hasto make a choice between an anatomic and a preformed post. The restoration withan anatomic post usually requires more than 1 visit. A semidirect procedure allowsthe fabrication of a more anatomic post. The fabrication of an anatomic post reducesthe thickness of the cement layer, which may be beneficial, as debonding is more aptto occur with a substantial layer of cement.22 Because inadequate post stiffnessresults in increased deformation of the post and localization of stress, the increasedthickness of the anatomic post in the coronal area reduces the chance of marginalfailure. Fiber posts also have demonstrated loss of flexural strength when theyundergo cyclic loading and thermocycling. One of the drawbacks with any prefabricated post system is the removal of addi-tional tooth structure to accommodate the post. In addition, a curved canal wouldpreclude use of a conventional post. A novel technique has been suggested to
406 Trushkowsky overcome these problems. StickTeck (Turku, Finland) has a system of glass fibers (everStick) that are impregnated with a semi-interpenetrating polymer network (IPN). An IPN network consists of a polymer with 2 or more networks that are not covalently bonded to each other. A semi-IPN network consists only of 1 network and a linear polymer. The everStick dowel consists of a matrix of a multiphase of bisphenol A diglycidy- lether methacrylate that is diffused into a linear phase of polymethyl methacrylate (PMMA). A PMMA outer layer surrounds this bundle to increase the adhesive proper- ties of the post. A light-curing bonding resin is then applied to the fiber bundle that was preimpregnated with PMMA and partially dissolves it. A result of this step is the crea- tion of grooves and undercuts that enhance micromechanical bonding. Polymerization results in the monomers forming a cross-link between the cross-linked semi-IPN poly- mer and phases of the linear polymer.23 This post system also does not depend on matching drills and provides the best fit of the available post space. Most fiber reinforced composite posts consist of a resin matrix glass or quartz fibers surrounded by a resin matrix. Quartz fibers have a greater tensile strength than glass fibers. The amount of fibers, their density, and their ability to bond to the resin matrix vary in each system, and consequently, so do their strengths.24 The resin matrix usually consists of an epoxy resin designed to withstand compressive stresses and absorb stresses in the entire system while the fibers supply tensile strength.25 Adhesion to the Post The ability of the fiber post to resist dislodgement is predicated on the adhesive, the luting material, and the cementation procedure.26 Adhesive composite cements that are recommended for use have the same elastic modulus as that of the post and dentin. Posts cemented with composite cements exhibit enhanced retention, and the roots are more fracture resistant because of more uniform stress distribution.27 Failure can also be attributed to inadequate marginal adaptation and subsequent orthograde contam- ination of the apical terminus.27 Adhesion between the post, core, and dentin are medi- ated by the composite resin cement. Despite the many techniques that have been introduced for improving the bond at the post-core interface, breakdown of the bond between the post and resin cement/dentin interface is often the cause of failure.28 Silane has been recommended to increase bond strength of posts. Fiber-reinforced posts that have highly cross-linked polymers in the matrix do not have functional groups that can chemically interact with silane. The DT Light-Post (Bisco, Schaum- burg, IL, USA) has no functional groups that can react with silane, but Style Post (Metalor Dental AG, Bienne, Switzerland) contains hydroxyl (-OH) groups on the surface of the silicate fiber. These groups can form covalent bonds with the silanol group of the silane coupling agent.29 Airborne particle abrasion with 50-mm aluminum oxide at 2.8 bar (0.28 MPa) pressure for 5 seconds has also been shown to increase surface area and minimize damage.30 Self-adhesive cements have been promoted as being simpler and less technique sensitive, but some of them demineralize the dentin, and the depth of resin penetration is not equivalent. In addition, residual acidic monomers may be present, reducing adhesion capabilities.31 The bonding method of self-adhesive cements involves both chemical interaction and micromechanical interlocking with the substrate. Self- adhesive cements work as dual-cure materials, and the chemical reaction is accom- plished by light irradiation. Some studies have indicated lower bond strengths and reduced mechanical properties when the cements are only autocured.32 This may present a problem, especially in the apical portion, as it is difficult to get light to pene- trate to the deepest apical areas.33 Light scattering in the resin cement is the result of
Restoring Endodontically Treated Teeth 407shadowing from tooth structure and the post.34 Dual-cured resin cements and adhe-sive systems are usually recommended as combining self-curing and light-curing.Despite the use of 2 initiation systems by some products, adequate light transmissionis needed to get light activation and the best results.35 Translucent glass or quartz fiberposts allow more transmission of light into the root canal space, resulting in increasedcure depth.36 Despite this increased depth of cure, the light transmission is still lessthan 40% of the incident light.37 It seems the amine in the base and the peroxide inthe catalyst cannot react adequately in the self-cure mode. Although these activationmodes are independent, light activation is required to increase the conversionrate.38,39 If self-etch adhesives are used with self- or dual-cure composite luting mate-rials, there may be an unfavorable reaction between the acidic resin monomers andthe tertiary amines that are used in the self-cure systems, resulting in inadequate poly-merization and poor bonding. However, if the acidic adhesives are fully cured, thisincompatibility would be mitigated. The amount of light and the duration of exposureare critical in reducing the adverse effects of uncured acidic monomers of one-stepself-etch adhesives. The mechanical properties of dual-cure adhesives are affectedby the duration and amount of light.39,40 The needed light energy is affected by the intensity and duration of the light. Aksorn-muang and colleagues41 found that extending the curing time from 10 to 30 secondsincreased bond strength by almost 3 times. Because light absorption weakens withincreasing cross-sectional distance from the irradiated surface, light at the apicalregion of a root canal would be greatly reduced.Adhesion to Intraradicular DentinBonding to intraradicular dentin is erratic. The predentin is a layer that consists ofunmineralized organic matrix that lines the deepest pulpal portion and has varyingwidth. The predentin is removed during instrumentation, sodium hypochlorite irriga-tion, and then by burs used to create the post space. The substrate remaining is miner-alized intraradicular dentin. This dentin contains tubules extending from the pulp to thetooth periphery.42 Intraradicular dentin is similar to coronal dentin, as it containstubules extending from the pulp to the periphery.42 The number of tubules decreasestoward the apical region, and the ratio between the peritubular and intertubular dentinchanges considerably from the apical to the coronal third.43 Therefore, peritubulardentin infiltration and resin tag formation decrease and intertubular dentin impregna-tion increases closer to the apex.44 Theoretically, the increased amount of intertubulardentin present for hybridization should increase bond strength in the apical one-third,but most studies have demonstrated a reduced bond strength in the apical one-thirdand diminished hybrid layer.42 The reduced bond strength may possibly be attributedto a negative C-factor.45 The variety of material used in an endodontic procedure may also reduce the abilityof the clinician to obtain a clean post space. The preparation of the post space withpost drills creates a thick smear layer, which consists of debris, sealer, and gutta-percha that reduce the bonding of the post to the intraradicular dentin.46 The postspace should ideally have clean dentinal surfaces to achieve optimal bonding withresin cement.47 The use of ethylenediaminetetraacetic acid and ultrasonic instrumen-tation has been suggested to clean the canal, but the bond strength is correlated to thebonding technique used. The use of etch-and-rinse or self-etch creates differentresults.48 Methacrylate resins shrink as they polymerize, resulting in shrinkage stress.The shrinkage stress is also related to the cavity configuration (C-factor). The C-factoris the ratio of bonded to unbounded surface areas in a restoration. If the C-factor ishigh, the stress development may exceed the bond strength of the bonding agent
408 Trushkowsky used.49,50 In a class I cavity, configuration of the C-factor is 5, as there are 5 times more bonded surfaces than unbounded surfaces. The post space can be considered as a deep narrow class I cavity preparation, and because the unbonded surface is small, there is insufficient stress relief by flow.51 Bouillaguet and colleagues52 found that C-factors in post spaces can exceed 200. SUMMARY The fracture resistance of endodontically treated teeth restored with a fiber post and a composite resin core is better than a tooth restored with a metal post.53 The wide variety of ceramic crowns used for an anterior restoration require a post and core that do not detract from the aesthetics that can be achieved with these restorations. Thin tissue biotype and a high smile line would benefit from the aesthetic potential of a fiber post and lack of a root discoloration. REFERENCES 1. Bittner N, Hill T, Randi A. Evaluation of a one-piece milled zirconia post and core with different post-and-core systems: an in vitro study. J Prosthet Dent 2010; 103(6):369–79. 2. Azer SS, Ayash GM, Johnston WM, et al. Effect of esthetic core shades on the final color of IPS Empress all-ceramic crowns. J Prosthet Dent 2006;96(6): 397–401. 3. Zalkind M, Hochman N. Esthetic considerations in restoring endodontically treated teeth with posts. J Prosthet Dent 1998;79(6):702–5. 4. Carossa S, Lombardo S, Pera P, et al. Influence of posts and cores on light trans- mission through different all-ceramic crowns: spectrophotometric and clinical evaluation. Int J Prosthodont 2001;14(1):9–14. ¨ ¨ 5. Deger S, Akgungor G, Caniklioglu B. An alternative method for fabricating a custom-made metal post with a ceramic core. Dent Traumatol 2005;21(3): 179–82. 6. Vichi A, Ferrari M, Davidson CL. Influence of ceramic and cement thickness on the masking of various types of opaque posts. J Prosthet Dent 2000;83(4):412–7. 7. Nakamura T, Saito O, Fuyikawa j, et al. Influence of abutment substrate and ceramic thickness on the colour of heat-pressed ceramic crowns. J Oral Rehabil 2002;29(9):805–9. 8. Michalakis KX, Hirayama H, Sfolkos J, et al. Light transmission of posts and cores used for the anterior region. Int J Periodontics Restorative Dent 2004;24(5): 462–9. 9. de Rouffignac M, de Cooman J. Aesthetic all-porcelain anterior restorations. Pract Periodonics Aesthet Dent 1992;4(8):9–13. 10. Morgano SM, Rodrigues AH, Sabrosa CE. Restoration of endodontically treated teeth. Dent Clin North Am 2004;48(2):397–416. 11. Cheung W. A review of the management of endodontically treated teeth; post, core and the final restoration. J Am Dent Assoc 2005;136(5):611–9. 12. Signore A, Bendicenti S, Kaitsas V, et al. Long-term survival of endodontically treated, maxillary anterior teeth restored with either tapered or parallel-sided glass-fiber posts or full-ceramic crown coverage. J Dent 2009;37(2):115–21. 13. Sorensen JA, Martinoff JT. Edodontically treated teeth as abutments. J Prosthet Dent 1985;53(5):631–6. 14. Theodosopoulou JN, Chochlidakis KM. A systematic review of dowel (post) and core materials. J Prosthodont 2009;18(6):464–72.
Restoring Endodontically Treated Teeth 40915. Peroz I, Blankenstein F, Lange KP, et al. Restoring endodontically treated teeth with post and cores: a review. Quintessence Int 2005;36(9):737–46.16. Dietschi D, Duc O, Krejci I, et al. Biomechanical considerations for the restoration of endodontically treated teeth: a systematic review of the literature. Part I. Composition and micro and macrostructure alterations. Quintessence Int 2007; 38(9):733–43. ¨ ¨17. Meyenberg KH, Luthy H, Scharer P. Zirconia posts a new all-ceramic concept for nonvital abutment teeth. J Esthet Dent 1995;7(2):73–80. ¨18. Stricker EJ, Gohring TN. Influence of different posts and cores on marginal adap- tation, fracture resistance and fracture mode of composite resin crowns on human mandibular premolars. An in-vitro study. J Dent 2006;34(5):326–35.19. Bakke M, Holm B, Jensen BL, et al. Unilateral, isometric bite force in 8–68 year old women and men related top occlusal factors. Scand J Dent Res 1990; 98(2):148–58.20. Morgano SM, Brackett SE. Foundation restorations in fixed prosthodontics: current knowledge and future needs. J Prosthet Dent 1999;82(6):643–57.21. Borracchini A, Ferrari M. SEM evaluation of the cement layer thickness after luting two different posts. J Adhes Dent 2005;7(30):235–40.22. Ferrai M, Vichi A, Mannocci F, et al. Retrospective study of the clinical perfor- mance of fiber posts. Am J Dent 2000;13(Spec No):9B–13B.23. Al-Tayyan MH, Watts DC, Kurer HG, et al. Is a “flexible” glass-bundle dowel system as retentive as a “rigid” quartz fiber dowel system? J Prosthodont 2008;17(7):532–7.24. Grinding S, Goracci C, Monticelli F, et al. Fatigue resistance and structural char- acteristics of fiber posts: three point bearing test and SEM evaluation. Dent Mater 2005;21(2):75–82.25. Seefield F, Wentz HJ, Ludwig K, et al. Resistance to fracture and structural char- acteristics of different fiber reinforced post systems. Dent Mater 2007;23(3): 265–71.26. D’Arcangelo C, Zazzeroni S, D’Amario M, et al. Bond strength of three types of fibre-reinforced post systems in various regions of root canals. Int Endod J 2008;41(4):322–8.27. Zicari F, Couthino E, De Munck JH, et al. Bonding effectiveness and sealing ability of fiber-post bonding. Dent Mater 2008;24(7):967–77.28. Vichi A, Mannocci F, Mason PN. Retrospective study of clinical performance of fiber posts. Am J Dent 2000;13(Spec No):9B–13B.29. Kern M, Thompson VP. Sandblasting and silica coating of glass-infiltrated alumina ceramic; volume loss, morphology, and changes in surface composition. J Prosthet Dent 1994;71(5):453–61.30. Balbosh A, Kjern M. Effect of surface treatment on retention of glass-fiber endodontic posts. J Prosthet Dent 2006;95(3):218–23.31. Mazzitelli C, Monticelli F. Evaluation of the push-out bond strength of self- adhesive resin to fiber posts. International Dentistry SA 2009;11(6):54–60.32. Radovic I, Monticelli F, Goracci C, et al. Self adhesive resin cements: a literature review. J Adhes Dent 2008;10(4):251–8.33. LeBellk AM, Tanner J, Lassila LV, et al. Depth of light-initiated polymerization of glass fiber-reinforced composite in a simulated root canal. Int J Prothodont 2003;16(4):403–8.34. Faria e Silva AL, Arias VG, Soares LE, et al. Influence of fiber-post translucency on the degree of conversion of a dual-cured resin cement. J Endod 2007;33(3): 303–5.
410 Trushkowsky 35. Roberts HW, Leonard DL, Vanderwalle KS, et al. The effect of a translucent post on resin composite depth of cure. Dent Mater 2004;20(7):617–22. 36. Yoldas O, Alacam T. Microhardness of composites in simulated root canals cured ¸ with light transmitting posts and glass-fiber reinforced composite posts. J Endod 2005;31(2):104–6. 37. Teixeira EC, Teixeira FB, Piasick JR, et al. An in vitro assessment of prefabricated fiber post systems. J Am Dent Assoc 2006;137(7):1006–12. 38. Braga RR, Cesar PF, Gonzaga CC. Mechanical properties of resin cements with different activation modes. J Oral Rehabil 2002;29(3):257–62. 39. El-Badrawy WA, El-Mowafy OM. Chemical versus dual curing of resin inlay cements. J Prosthet Dent 1995;73(6):515–24. 40. Tanoue N, Koishi Y, Atsuta M, et al. Properties of dual-curable luting composites polymerized with single and dual curing modes. J Oral Rehabil 2003;30(10): 1015–21. 41. Aksornmuang J, Nakajima M, Panyayong W, et al. Effects of photocuring strategy on bonding of dual-cure one step self-etch adhesive to root canal dentin. Dent Mater J 2009;28(2):133–41. 42. Ferrari M, Mannocci F, Vichi A, et al. Bonding to root canal: structural character- istics of the substrate. Am J Dent 2000;13(5):255–60. 43. Mjor IA, Smith MR, Ferrari M, et al. The structure of dentine in the apical region of human teeth. Int Endod J 2009;34(5):346–53. 44. Mannocci F, Pilecki P, Bertelli E, et al. Density of dentinal tubules affects the tensile strength of root dentin. Dent Mater 2004;20(30):293–6. 45. Breschi L, Mazzoni A, Ferrari M. Adhesion to intra-radicular dentin. In: Ferrari M, Breschi L, Grandini S, editors. Fiber posts and endodontically treated teeth: a compendium of scientific and clinical perspectives. Wendywood (SA): Modern Dentistry Media; 2008. p. 15–37. 46. Goracci C, Sadek FT, Fabianelli A, et al. Evaluation of the adhesion of fiber posts to intradicular dentin. Oper Dent 2005;30(5):627–35. 47. Boone KJ, Murchison DF, Schindler WG, et al. Post retention: the effect of sequence of post preparation, cementation time, and different sealers. J Endod 2001;27(12):768–71. 48. Coniglio I, Magni E, Goracci C, et al. Post space cleaning using a new nickel tita- nium endodontic drill combined with different cleaning regimens. J Endod 2008; 34(1):83–6. 49. Feilzer AJ, DeGee AJ, Davidson CL. Setting stress in composite resin in relation to configuration of the restoration. J Dent Res 1987;66(11):1636–9. 50. Tay FR, Loushine RJ, Lambrechts P, et al. Geometric factors affecting dentin bonding in root canals: a theoretical modeling approach. J Endod 2005;31(8): 584–9. 51. Goracci C, Fabianelli A, Sadek FT, et al. The contribution of friction to the dislo- cation resistance of bonded fiber posts. J Endod 2005;31(8):608–12. 52. Bouillaguet S, Troesch S, Wataha JC, et al. Microtensile bond strength between adhesive cements and root canal dentin. Dent Mater 2003;19(3):199–205. 53. Hayashi M, Sugeta A, Takahashi Y, et al. Static and fatigue fracture resistances of pulpless teeth restored with post-cores. Dent Mater 2008;24(9):1178–86.